## Magnetic Weyl semimetals

Weyl semimetals (WSMs)—materials that host exotic quasiparticles called Weyl fermions—must break either spatial inversion or time-reversal symmetry. A number of WSMs that break inversion symmetry have been identified, but showing unambiguously that a material is a time-reversal-breaking WSM is tricky. Three groups now provide spectroscopic evidence for this latter state in magnetic materials (see the Perspective by da Silva Neto). Belopolski *et al.* probed the material Co_{2}MnGa using angle-resolved photoemission spectroscopy, revealing exotic drumhead surface states. Using the same technique, Liu *et al.* studied the material Co_{3}Sn_{2}S_{2}, which was complemented by the scanning tunneling spectroscopy measurements of Morali *et al.* These magnetic WSM states provide an ideal setting for exotic transport effects.

*Science*, this issue p. 1278, p. 1282, p. 1286; see also p. 1248

## Abstract

Topological matter is known to exhibit unconventional surface states and anomalous transport owing to unusual bulk electronic topology. In this study, we use photoemission spectroscopy and quantum transport to elucidate the topology of the room temperature magnet Co_{2}MnGa. We observe sharp bulk Weyl fermion line dispersions indicative of nontrivial topological invariants present in the magnetic phase. On the surface of the magnet, we observe electronic wave functions that take the form of drumheads, enabling us to directly visualize the crucial components of the bulk-boundary topological correspondence. By considering the Berry curvature field associated with the observed topological Weyl fermion lines, we quantitatively account for the giant anomalous Hall response observed in this magnet. Our experimental results suggest a rich interplay of strongly interacting electrons and topology in quantum matter.

Topological phases of matter can host analogs of particles relevant for high-energy physics and may enable fresh pathways for the application of quantum materials (*1*–*10*). To date, most topological phases have been discovered in nonmagnetic materials (*6*–*8*), thus limiting their magnetic field tunability, as well as their electronic and magnetic functionality. Identifying and understanding electronic topology in magnetic materials has the potential to lead to the discovery of novel magnetic responses that may be used for future spintronics technologies. Recently, several magnets were found to exhibit a large anomalous Hall response in transport, which has been linked to a large Berry curvature in their electronic structures (*11*–*15*). However, it remains largely unclear in experiment whether the Berry curvature originates from a topological band structure, such as Dirac and Weyl points or node lines. In particular, there is no direct visualization of a topological magnetic phase demonstrating a bulk-boundary correspondence with associated anomalous transport. In this study, we use angle-resolved photoemission spectroscopy (ARPES), ab initio calculation, and transport to explore the electronic topological phase of the ferromagnet Co_{2}MnGa (*10*). We observe node lines that we identify as Weyl fermion lines, along with drumhead surface states. We find that the Weyl lines concentrate the Berry curvature, accounting for the giant intrinsic anomalous Hall response in Co_{2}MnGa.

Topological phases can be categorized by the dimensionality of the band touching into topological insulators, node point semimetals, and node line semimetals (*8*, *16*–*18*). Node points are often further subcategorized as Dirac points, Weyl points, and other exotic point touchings (*8*). Analogously, node lines may include Dirac lines (fourfold degenerate), Weyl lines (twofold degenerate), and possibly other one-dimensional (1D) band crossings (*19*–*21*). Node lines may be protected by crystal mirror symmetry, giving rise to drumhead surface states (*9*, *17*, *18*, *22*–*25*). Co_{2}MnGa takes a cubic face-centered Bravais lattice (Fig. 1A), space group *26*) and Curie temperature *T*_{C} = 690 K (Fig. 1B) (*27*), indicating broken time-reversal symmetry. This suggests that all bands are generically singly degenerate and that mirror symmetry may give rise to twofold-degenerate node lines. In a detailed theoretical analysis, we studied the band structure of Co_{2}MnGa by ab initio calculation, neglecting spin-orbit coupling (SOC). We found that the ferromagnetic exchange splitting drives a phase with two majority spin bands near the Fermi level that exhibit twofold degeneracies on the mirror planes (*18*). These degeneracies, which arise from a crossing of bands with opposite mirror eigenvalues, form three families of Weyl lines (Fig. 1C and fig. S10), which are pinned to each other, forming a nodal chain; some of them further form Hopf-like links with one another (*10*). The predicted Weyl lines are protected only when the SOC is strictly zero, but numerical results in the presence of SOC suggest that the gap opened is negligible (fig. S9).

Motivated by these considerations, we investigate Co_{2}MnGa single crystals by ARPES. We focus first on the constant-energy surfaces at different binding energies, *E*_{B}. We readily observe a feature that exhibits an unusual evolution from a < shape (Fig. 1, D and E) to a dot (Fig. 1F) to a > shape (Fig. 1, G and H). This feature suggests that we observe a pair of bands that touch at a series of points in momentum space. As we shift downward in *E*_{B}, the touching point moves from left to right (black guides to the eye in Fig. 1, D to H), and at certain *E*_{B} (Fig. 1F) the spectral weight appears to be dominated by the crossing point. This series of momentum-space patterns is characteristic of a node line (Fig. 1I). For the constant-energy surfaces of a node line, as we slide down in *E*_{B}, the touching point slides from one end of the node line to the other, gradually zipping closed an electron-like pocket (upper band) and unzipping a hole-like pocket (lower band). To better understand this result, we consider *k _{x}*, in-plane crystal momentum) cuts passing through the node line feature (Fig. 2A). On these cuts, we observe a candidate band crossing near

*k*and moves downward in energy as we cut further from

_{y}*k*). We can fit the candidate band crossing with a single Lorentzian peak, suggestive of a series of touching points between the upper and lower bands (fig. S13). Taking these fitted touching points, we can in turn fit the dispersion of the candidate node line to linear order, obtaining a slope

_{y}*k*, the bands disperse linearly in energy away from the touching points. Taken together, our ARPES results suggest the presence of a node line at the Fermi level in Co

_{y}_{2}MnGa.

To better understand our experimental results, we compare our spectra with ab initio calculations of Co_{2}MnGa in the ferromagnetic state (*10*). We consider the spectral weight of bulk states on the (001) surface and study an *28*). At *X* point of the bulk Brillouin zone (blue node line in fig. S10). According to our earlier theoretical analysis, the node line resides on the *M _{xy}* (and equivalent) mirror planes (

*10*). This node line is a Weyl line, in the sense that it is a twofold-degenerate band crossing extended along one dimension (

*19*–

*21*). It is predicted to be pinned to a second, distinct Weyl line, forming part of a nodal chain. To compare experiment and theory in greater detail, we plot the calculated dispersion of the Weyl line against the dispersion as extracted from Lorentzian fits of ARPES data (fig. S15). We observe a hole-doping of experiment relative to theory of

_{2}MnGa.

Having considered the blue node line marked in Fig. 2A, we search for other node lines in our data. We compare an ARPES spectrum (Fig. 2, C and D) to an ab initio calculation of the surface spectral weight of bulk states, taking into account the observed effective hole-doping of our sample (Fig. 2E). In addition to the blue Weyl line (labeled in Fig. 2, D and E, as *a*), we observe a correspondence between three other features in experiment and theory, marked as *b*, *c*, and *d*. To better understand the origin of these features, we consider all of the predicted Weyl lines in Co_{2}MnGa (*10*) and plot their surface projection with the energy axis collapsed (Fig. 2F). We observe a correspondence between *b* in the ARPES spectrum and the red Weyl line. Similarly, we see that *c* and *d* match with predicted yellow Weyl lines. To further test this correspondence, we look again at our ARPES constant-energy cuts and find that *d* exhibits a transition from a < shape to a > shape, which suggests a node line (figs. S16 and S17). The comparison between ARPES and ab initio calculation suggests that an entire network of magnetic Weyl lines is realized in Co_{2}MnGa.

Next we explore the topological surface states. We study the ARPES spectrum along *k _{a}*, as marked by the green line in Fig. 3F. On this cut we observe three cones (red arrows in Fig. 3A) that are consistent with the yellow Weyl lines. Notably, we also observe a pair of states that appear to connect one cone to the next (Fig. 3, A to C). Moreover, these extra states consistently terminate on the candidate yellow Weyl lines as we vary

*k*(fig. S20). We further carry out a photon energy dependence study and discover that these extra states do not disperse with photon energy from

_{b}*h*ν = 34 to 48 eV (

*h*, Planck’s constant; ν, frequency), suggestive of a surface state (Fig. 3G). In ab initio calculation, we observe a similar pattern of yellow Weyl lines pinning a surface state (Fig. 3E) (

*28*). These observations suggest that we have observed a drumhead surface state stretching across Weyl lines in Co

_{2}MnGa. The pinning of the surface states to the cones further points to a bulk-boundary correspondence between the bulk Weyl lines and the drumhead surface state dispersion.

Now that we have provided spectroscopic evidence for a magnetic bulk-boundary correspondence in Co_{2}MnGa, we investigate the relationship between the topological node lines and the anomalous Hall effect (AHE). We study the Hall conductivity *T* and extract the anomalous Hall conductivity *11*, *12*). To understand the origin of the large AHE, we study the scaling relation between the anomalous Hall resistivity, *29*–*31*). When we plot *33*). From the linear fit, we find that the intrinsic Berry curvature contribution to the AHE is *28*). Next we investigate the Berry curvature up to a given binding energy to predict _{2}MnGa.

Our ARPES and corresponding transport experiments, supported by ab initio calculation, provide evidence for magnetic Weyl fermion lines and drumhead topological surface states in the room temperature ferromagnet Co_{2}MnGa. With 1651 magnetic space groups and thousands of magnets in 3D solids, the experimental methodology of transport-bulk-boundary exploration established in this work can be a valuable guideline in probing and discovering other topological phenomena on the surfaces and the bulk of magnetic or strongly correlated electronic materials.

## Supplementary Materials

science.sciencemag.org/content/365/6459/1278/suppl/DC1

Materials and Methods

Supplementary Text

Figs. S1 to S22

This is an article distributed under the terms of the Science Journals Default License.

## References and Notes

**Acknowledgments:**We thank D. Lu and M. Hashimoto at Beamlines 5-2 and 5-4 of the Stanford Synchrotron Radiation Lightsource (SSRL) at the SLAC National Accelerator Laboratory, CA, USA, and J. Denlinger at Beamline 4.0.3 and S.-K. Mo at Beamline 10.0.1 of the Advanced Light Source (ALS) at Lawrence Berkeley National Laboratory (LBNL), CA, USA, for support.

**Funding:**Work at Princeton University is supported by the U.S. Department of Energy (DOE) under Basic Energy Sciences, grant no. DOE/BES DE-FG-02-05ER46200. I.B. acknowledges the support of the Harold W. Dodds Fellowship of Princeton University. The work at Northeastern University was supported by DOE, Office of Science, Basic Energy Sciences grant no. DE-FG02-07ER46352 and benefited from Northeastern University’s Advanced Scientific Computation Center (ASCC) and the NERSC supercomputing center through DOE grant no. DE-AC02-05CH11231. Use of the Stanford Synchrotron Radiation Lightsource (SSRL), SLAC National Accelerator Laboratory, is supported by the U.S. Department of Energy, Office of Science, Office of Basic Energy Sciences, under contract no. DE-AC02-76SF00515. This research used resources of the Advanced Light Source, which is a DOE Office of Science User Facility under contract no. DE-AC02-05CH11231. K.M., B.E., and C.F. acknowledge the financial support by the ERC Advanced Grant no. 291472 “Idea Heusler” and 742068 “TOPMAT.” STM characterization of samples was supported by the Gordon and Betty Moore Foundation (GBMF4547/Hasan). M.Z.H. acknowledges support from the Miller Institute of Basic Research in Science at the University of California at Berkeley and Lawrence Berkeley National Laboratory in the form of a Visiting Miller Professorship during the early stages of this work. M.Z.H. also acknowledges visiting scientist support from IQIM at the California Institute of Technology.

**Author contributions:**The project was initiated by I.B., K.M., C.F., and M.Z.H. I.B. and D.S.S. carried out ARPES measurements and analyzed ARPES data with assistance from G.C., J.Y., S.S.Z., T.C., N.S., H.Z., G.B., D.M., M.L., S.-Y.X., and M.Z.H. K.M. synthesized the single-crystal samples and carried out the transport and magnetization measurements with assistance from B.E. I.B. and K.M. analyzed the transport data with assistance from G.C. and T.C. G.C. performed first-principles calculations and theoretical analysis with assistance and guidance from B.S., G.B., X.Z., S.-M.H., B.W., T.-R.C., S.-Y.X., A.B., and H.L. The project was supervised by C.F., H.L., and M.Z.H. All authors discussed the results and contributed to writing the manuscript.

**Competing interests:**The authors declare no competing interests.

**Data and materials availability:**The data presented in this work are available on Zenodo (

*34*).